Both electrical and mechanical wear contribute to the loss of contact material. Electrical wear due to arcing phenomena depends on the form of the contacts, a.c.- or d.c.-switching, contact speed, and contact pressure. Mechanical wear due to friction depends on the nature of the material, the form of the contacts, their relative movement, and the pressure between them. Decrease of contact wear, either by eliminating one of the causes of wear or by redesigning the contact mechanism, is of extreme importance in increasing the reliability of contacts.
ZUSAMMENFASSUNG Der Schaltstiick-stoff geht durch elektrischen und mechanischen Verschleiss verloren. Der eleklrisch Verschleiss, der unvermeidlich ist, wird durch die Einwirkung des Lichtbogens verursacht: er wird ebenfalls beeinflusst durch Elektrodenform, Kontaktdruck-kraft, Schaltgeschwindigke~t, Prellsc.hIag und Stromart: Gleich- oder Wechselstrom. Die mechanische Abnutzung wird beeinflusst durch Reibung zwischen den Kontaktflachen, Werkstoff, Elektrodenform und Kontaktdruckkraft. Es ist sehr wichtig nach Verminderung des Kontaktverschleisses zu streben entweder durch Aufhebung der Verschleissursachen oder durch Neu-entwurf der Kontaktsysteme, damit die Schaltsttick-lebensdauer und die Betriebssicherheit des Kontaktes erhijht wird. Aus einer Analyse der Verschleissursachen folgen MitteI zur Verbesserung der Kontaktkonstruktion.
Satisfactory operation and lifetime of electric switchgear depend largely on the quality of the electrical contacts. All places through which electric current passes from one conductor to another are electrical contacts. Usually differentiation is made between fixed contacts, where the current only passes and which cannot be loosened except with tools, and temporary or switch contacts, where a current is switched on and off. From the point of view of wear, only the switch contacts are important. When the circuit is broken electrical energy is set free at the switch contacts and arcing has a destructive effect on the material. So it is quite natural that after a certain number of operations the quality of the contacts should decrease and replacement be necessary. But this type of wear should be not accepted as inevitable; on the contrary, by improvements in the design the lifetime can be increased and replacement postponed for as long as possible. Eeferences
M. G. DIEHL
When studying wear of electrical contacts, it will be evident that there is a complex of phenomena, mixed up in such a way that it is very difficult to examine the various conditions separately.
A contact is said to be worn out when its form has changed so much that the contact can no longer perform its function. A certain mechanical force, derived from a compressed or bent spring, keeps the contacts in the closed position. No attention has been paid to a possible decrease of the elastic properties, this being a problem of erroneous dimensions. Erosion of contact material diminishes the contact pressure; in the extreme case the contacts touch only slightly but the wear has then greatly exceeded its maximum value. A contact is already worn out when, because of the decreased contact pressure, the contact resistance is so much higher than normal that the temperature rise surpasses a certain limit on passage of current. This wear can be examined indirectly by measurement as shown in Fig. I ; the limits should be mentioned by the manufacturer.
Contacts are worn out when A is reduced to minimum given value.
Although the contact resistance depends to a great extent on the contact pressure, the condition of the material surfaces also influences the resistance. In addition to the wear, which in this consideration is equal to the loss of material, the increase in resistance caused by oxidation causes a fall in quality, which is also marked by an extra temperature rise. Such a contact is not then worn out, but it is no longer usable for its purpose. CAUSES
When analysing the problem of wear of electrical contacts, various causes must be taken into account: (a) electrical phenomena, (b) mechanical influences, (c) conditions of operation. Although chemical reactions may have an effect they are left out in this consideration because they influence the main causes only indirectly. References p. 376
WEAR OF ELECTRICAL
Since switches vary so much in design and construction, several conditions influence the wear, each in its own way. To obtain a more fundamental view of the wear of contacts it is necessary to study the problem apart from the type of construction involved. A study of the switch construction will reveal which factors of wear are connected with the construction and which dominate. Should this fundamental research be omitted, there is a good chance that alterations in design that, incidentally, bring about an improvement in results will not be made use of as a basis for new or modified designs. The quality of an electrical contact is determined by the following factors: contact form ; contact pressure ; contact material, as far as suitability for passing current is concerned; type and strength of current and voltage: power factor; operating speed; relative movement after touch; bounce of contacts; type of switch, with regard to making and breaking the circuit and duration of contacts. In order to examine the effect of one of these factors on the phenomenon of wear a situation should be chosen in which the effect of all other factors will be eliminated or so much restricted that reproducible data can be obtained. An investigation of a special construction in which several factors play a part seldom gives results that are of general use.
Contact material is lost owing to electrical phenomena, viz. when switching. As soon as an arc has been formed (this being a conducting path through the medium, either air or oil) the material will be vaporized or burnt, since the temperature of the arc is some thousands of degrees centigrade. As is known, an arc is formed when the distance between the contacts at breaking is so small that an electric breakdown of the medium is possible, and moreover when the current is interrupted by ionization of the medium. Some loss of contact material must be expected at each sparking or arcing, even if this takes only a short time. Generally, these quantities are small, although they depend on the load; after a great number of operations the wear can be determined by weighing the contacts. The wear is usually stated in g/rooo operations (or multiples thereof); I operation = I closing + I opening of the contact. (b) Contact
Although at first sight contacts seem to have a large variety of forms, there are some elementary shapes (see Fig. z) to which all types belong: References p. 376
A. spherical against spherical : 1%. cylindrical against cylindrical ; (‘. spherical against plane : 1). cylindrical against plane ; E. plane against plane. If relative movement of the contacts after they first make contact is excluded, no mechanical friction will occur and all loss of material will be caused by electrical phenomena. A simple calculation will show how the loss of material depends on the flattening 1-f of the contacts or the increase of the contact opening. Here it is assumed that per average operation an equal quantity of material is lost. The graphs of Fig. 2 have been made for contacts with a radius of curvature R = 5 mm. These prove that very curved surfaces, especially in the beginning, lose material more quickly than surfaces that are less curved; the coaxially-mounted cylinders - where the surface is independent of the wear -- give the best results,
Fig. 2. Relatir~llship between flattening and erosion of material on various types of contact.
(c) Contact pressure As can easily be seen, the influence of the contact pressure on the wear is nil for the contacts without relative movement after contact is first made. The quality of the contact, however, is highly dependent on the mean pressure: if this increases, the contact resistance and the voltage drop decrease. As the pressure tends to increase at several points of contact the yielding point of the material will be exceeded, which means that the area of current passage will become larger. (d) Contact material In selecting a suitable material for electrical contacts attention should be given to the fact that low resistance to current is usually accompanied by good thermal conducRefet-encesp. 376
1 (1957/[email protected]
tivity. But a low contact resistance is in many cases incompatible with good resistance to electrical wear. Copper and silver show good current and heat conductivity,
copper is apt to form surface film, which increases the contact resistance. Tungsten shows good resistance both to electrical and mechanical wear, owing to its high melting point and hardness. In many applications a compromise has to be found between the conflicting requirements. (e) Nature
There is an important difference between the wear when using alternating or direct current. When d.c. is interrupted the arc characteristically remains more or less stable, unless the construction of the contacts prevents it. The longer the arc the greater the resistance. Ultimately, as the contact opening becomes wide enough the arC will break down. Moreover, the heat development of the surrounding air contributes to the vertical movement of the arc. Advantage is taken of the phenomenon by artificially enlarging the length of the arc during the raising movement, in order to stimulate a quick breakdown. Rapid extinction is obtained with the aid of a blow-out coil, the magnetic field of which exercises a force over the arc that can be seen as a moving conductor, which lengthens the arc and makes it break down earlier. Alternating current has an inherent advantage in this respect, in that the current at a frequency of 50 cycles/set is zero IOO times per second. After opening the contact the current is interrupted at the next zero value. Because the arc is of such short duration the influence of the electrical energy on the contact material is restricted. In this respect the wear in a.c. switches is considerably less than in d.c. switches. This does not mean that the characteristics of the load have no influence : the cos ~1between current and voltage, and thus the qualities of the load circuit, play a great part in the interrupting phenomena. MECHANICAL
The mechanical phenomena, which are closely connected with the design of the switch, can have a great influence and can be the cause of considerable wear. It is usually possible to reduce them to frictional wear. In a switch the unusual situation exists that metal parts are rubbing against each other without lubrication ; after a time this causes much loss of material. The contact pressure is more important for those contacts that still move after the first moment of contact. For in such cases two metal parts rub on each other, and it is not strange that this unlubricated or dry friction should cause a serious loss of material. (b) Contact
The contact arrangement and relative movement must be known before one can forecast the wear. There are usually two types of contact, viz. contact where after References p. 376
first touching the tips of the contacts move along t~h other with the full contact forcca until they come to a standstill, and contact where tliv mo\ing part of the contact rolls - and possibly also slides - along the fixed part of the contact. ‘I’hc principle of the rolling form of contact is, not to allow the point of first and last contact to coincide with the place of definite contact, so that the latter will not bc tlamagcxl R? the arc phenomena during switching. ‘Tests on wear without electric load on a specially constructed
(Fig. .$) have shown that during LOSS
4. 1.0~~ of material
References p. 376
of two sliding
copper blocks polish each other at first, but after a certain
the loss of material
WEAR OF ELECTRICAL CONTACTS
higher and the material
surfaces become very rough.
The higher the pressure is, the sooner this phenomenon appears (Fig. 4). Although this test gives only a rough view of the mechanical phenomena,
be expected that in practice - when a combination of mechanical and electrical phenomena exists - more favourable results will be obtained, since the attack of the surface by an arc nullifies
action of the contacts.
(c) Contact material Because of this considerable mechanical wear, contacts with a high rupturing capacity should be designed in such a way that there is a little relative movement. For switches that operate only seldom the mechanical friction is necessary in order to remove any possible surface film of oxide with poor conducting qualities, so that good contact and low contact resistance will be achieved. When silver, silver alloys, or silver-sintered contact materials are used mechanical friction is no longer essential since the silver oxide good conductor. There is no loss of material, because due to electrical phenomena alone. On this principle of contactors specially for a.c., having double-break wiping movement.
(formed by the arcing) is also a there is no friction, and wear is is based the present development contacts without any rolling or
Apparatus for uetermrnmg eroslon of contact material at different values of contact speed.
References p. 376
(a) Operating Although
when switching off a.c. the moment of definite interruption
appears to be the passage through zero, the operating from the point of view of wear. Again,
of the current
speed is also of some importance
speed will mostly
vary in the
switch itself. In order to check the influence of speed upon wear a special cam-operated contact
of circuit breaking. a certain
is used, where the operating
speed. If switching
there is a difference actual
wear. Moreover, an influence.
as two separate
speed of switching
on and switching
at the moment
that wear shows a definite
on and off are investigated
between the optimum
the vaiue of minimum
speed is the speed of the moving contact
on switching and the
Fig. 6 shows the relationship
Fig. 6. Relationship between electrical wear and contact speed.
ment, but the arrangement In a comparison vertically,
is made between horizontal
of the contact
of the wear on contacts
there is a real difference
in favour of the horizontal
clearest at small speeds of 5-50 mm/set. The duration upon the erosion of contact
and vertical contact
does play a part with regard to wear. and those moving
and this is
of the arc has a direct influence
and the sooner the arc phenomena
the smaller will be the loss. As a result of the heat effect of the arc and its rising moveReferences
WEAR OF ELECTRICAL
ment, there is also a rising movement replacement
of the surrounding
of warm ionized air by cold no-ionized
air; this contributes
air with higher disruptive
to the strength.
Naturally, the ventilation effect is less effective with a vertical switching motion than with a horizontal arc. Generally the mean difference in wear is of less significance for constructions magnets,
where the arc is extinguished
forcibly, as with the application
(c) Contact bounce Every time a contact is closed and opened, it is exposed to the disturbing influence as already described. In automatic switchgear, the greater part of which is electromagnetically operated, contact bounce is an extra source of wear. On closing the circuit the moving contact is suddenly arrested by the fixed contact. Owing contact before number in Fig. contact of the
to the kinetic energy of the mass moving with high speed, a rebounding of the breaks the circuit ; this phenomena is repeated several times in rapid succession making is definite. It will be clear that wear is more or less proportional to the of undesired interruptions. From a cathode ray oscillogram such as is given 7 it is possible to forecast the extra wear that may be expected in a given arrangement. In a more serious case the contact bounce may lead to welding contacts,
Fig. 7. Oscillogram
of current interruptions
due to contact
Without going further into the fundamental questions regarding the complicated arc phenomena, it appears that wear is a still more complex problem, because it is influenced not only by these phenomena but also by other factors. However, it is very Re/erences 9, 376
useful to trace the result of these factors, either separately
that on the basis of these facts it can be decided in which direction must be sought. In view of the considerable it is - quite independently important task to increase
decrease of wear
used in the technical
of the economic aspect of the loss of material their reliability by decrease of wear.
--- a very
R. HOLM, Die technische Pkysik der elektrischm Kmtakte, Nerlin, 1941, Stockholm, 1946. G. WINDRED, Electrical Contacts, London, 1940. S. G. ESKIN, Effect of contact opening speed on arc energy in a.~. switching, C;ex. Elec. NW., 42 (‘939) 81. M. G. DIEHL, Contactslijtage, Electvoteckniek, 24 (1946) 40. M. G. DIEHL, Mechanische slijtage van contactstukken, Elektvofechniek, 28 (rggo) 218. M. G. DIEHL, Invloed van de schakelsnelheid op de contactslijtage bij wisselstroomschakelaars, ~~ek~afeckn~ek, 3r (1953) 189. Received October 12, rg57 Accepted December 20, 1957